A Gradient-Field Pulsed Eddy Current Probe for Evaluation of Hidden Material Degradation in Conductive Structures Based on Lift-Off Invariance Yong Li 1, *, Haoqing Jing 1 , Ilham Mukriz Zainal Abidin 2 and Bei Yan 1 1

2

*

State Key Laboratory for Strength and Vibration of Mechanical Structures, Shaanxi Engineering Research Center of NDT and Structural Integrity Evaluation, Xi’an Jiaotong University, Xi’an 710049, China; [email protected] (H.J.); [email protected] (B.Y.) Leading Edge NDT Technology (LENDT) Group, Malaysian Nuclear Agency, 43000 Bangi, Kajang, Selangor, Malaysia; [email protected] Correspondence: [email protected]; Tel.: +86-29-8266-5721

Academic Editors: Ashutosh Tiwari and Bharati Tudu Received: 28 March 2017; Accepted: 22 April 2017; Published: 25 April 2017

Abstract: Coated conductive structures are widely adopted in such engineering fields as aerospace, nuclear energy, etc. The hostile and corrosive environment leaves in-service coated conductive structures vulnerable to Hidden Material Degradation (HMD) occurring under the protection coating. It is highly demanded that HMD can be non-intrusively assessed using non-destructive evaluation techniques. In light of the advantages of Gradient-field Pulsed Eddy Current technique (GPEC) over other non-destructive evaluation methods in corrosion evaluation, in this paper the GPEC probe for quantitative evaluation of HMD is intensively investigated. Closed-form expressions of GPEC responses to HMD are formulated via analytical modeling. The Lift-off Invariance (LOI) in GPEC signals, which makes the HMD evaluation immune to the variation in thickness of the protection coating, is introduced and analyzed through simulations involving HMD with variable depths and conductivities. A fast inverse method employing magnitude and time of the LOI point in GPEC signals for simultaneously evaluating the conductivity and thickness of HMD region is proposed, and subsequently verified by finite element modeling and experiments. It has been found from the results that along with the proposed inverse method the GPEC probe is applicable to evaluation of HMD in coated conductive structures without much loss in accuracy. Keywords: electromagnetic non-destructive evaluation; gradient-field pulsed eddy current probe; lift-off invariance; material degradation; inversion; coated conductive structures

1. Introduction Coated conductive structures of nonmagnetic materials involving Aluminum, Copper and Titanium, etc. can be widely found in industrial fields including aerospace, nuclear, transportation, chemical engineering, etc., and normally serve in corrosive and hostile environment. Therefore, in-service coated conductive structures are usually found subject to structural corrosion whose initial exhibition is material degradation within a localized region in the structure [1]. Even though the nonmetallic protection coating is deployed over the conductor surface, coated conductive structures are still vulnerable to material degradation especially hidden under the coating. The Hidden Material Degradation (HMD) severely undermines the integrity of conductive structures, since it can barely be detected or even monitored without removing the protection coating. As a result, it is indispensable to non-invasively monitor the development of HMD in terms of the material property and thickness of degradation region before the structural failure occurs.

Sensors 2017, 17, 943; doi:10.3390/s17050943

www.mdpi.com/journal/sensors

Sensors 2017, 17, 943

2 of 12

As one of the advanced eddy current techniques [2,3], Gradient-field Pulsed Eddy Current technique (GPEC) has been found to be advantageous in detection and evaluation of corrosion in metallic structures in terms of high inspection sensitivity and evaluation accuracy [4]. It could be one of the promising techniques for evaluation of HMD in coated conductive structures. Whereas, two critical inspection issues must be resolved before inspection probes based on GPEC (namely GPEC probes) are applied: (1) the coating thickness may vary, which causes the variation in the distance between the probe bottom and conductor surface (namely lift-off), and thus gives rise to the lift-off noise in testing signals; and (2) intricate calculation is needed for simultaneous evaluation of the conductivity and thickness of HMD. Lift-off Invariance (LOI) is a phenomenon which has been discovered from previous research regarding not only harmonic eddy current testing but also transient eddy current testing. It indicates that when the lift-off varies during the inspection of a conductor, the testing signals for various lift-off scenarios intersect [5–7]. The intersection point (namely LOI point) parameters including the LOI amplitude (Mloi , the signal magnitude at the intersection point) and LOI time (Tloi , the time instant of the intersection point) are believed to be immune to the lift-off variation whilst they merely vary with specimen properties [8,9]. Giguere et al. adopted Mloi of the LOI point found in pulsed eddy current testing signals for imaging of cracks in the rivets [10]. Tian et al. investigated Tloi of pulsed eddy current testing signals, and utilized it for evaluation of the lift-off and metal conductivity [11]. Therefore, the first issue could be resolved by using the LOI in signals from GPEC probes. However, to the authors’ knowledge, the research of LOI regarding GPEC has been barely conducted yet. Since parallel quantification of the conductivity and thickness of HMD in coated conductive structures is a typical inverse problem of eddy current testing, inverse schemes which are mostly based on deterministic approaches and utilized for defect reconstruction could be applied to resolve the second issue. Xie et al. established a deterministic-approach-based model integrating the conjugate gradient algorithm with a finite element model for retrieving the profile of the wall-thinning defect in steam generator tubes of nuclear power plants via eddy current testing [12]. Bai et al. proposed an inverse scheme for fast crack reconstruction based on transient slices and spectral components of pulsed eddy current signals [13]. Nevertheless, few researches have been carried out for investigation and implementation of an inverse scheme based on parameters of LOI point in testing signals from GPEC probes for simultaneous evaluation of HMD parameters including the conductivity and thickness of degradation region. In light of this, the GPEC probe for evaluation of HMD in coated planar conductors is intensively investigated in this paper. The closed-form expression of the testing signal from the GPEC probe is formulated based on the analytical modeling i.e., the Extended Truncated Region Eigenfunction Expansion [14]. The correlations of the amplitude and time instant of the LOI point (Mloi and Tloi ) in GPEC signals with the conductivity and thickness of HMD region are investigated through theoretical study. Based on this, in conjunction with Levenberg–Marquardt algorithm [15] a fast inverse method based on LOI of GPEC for quantitative assessment of HMD is proposed. The proposed inverse method is subsequently verified via finite element modeling and experiments. 2. Field Formulation of GPEC and Investigation of LOI 2.1. Field Formulation The structure of the GPEC probe is similar to that of pulsed eddy current testing except that magnetic sensors deployed in the excitation coil are used for measuring gradient magnetic field in lieu of absolute magnetic field. Suppose that a cylindrical GPEC probe consisting of an excitation coil for generation of incident magnetic field and magnetic sensor for sensing the net gradient field is deployed over a coated nonmagnetic conductor with HMD. The model is shown in Figure 1. It is assumed that the length and width of the HMD area are considerably larger than the outer diameter of the excitation

Sensors 2017, 17, 943

3 of 12

coil. Based on the analytical modeling [14,16], the GPEC signal concerning the z-direction gradient Sensors 2017, 17, 943 3 of 12 field of the z-component of net magnetic field is formulated as: h i ∞ ∂Bz Bµ0 N I (t)0 NI (t ) ai z a z − aia(z( z+ − a z a rχ, (aari r1 , ai r2 ) ) ) z a z a z 22ρ a − (1) ⊗ J a r e − e η ( t ) gz ( Bz ) = g z Bz = ( ) J a r e e ( t ) e e i e1 − e i 2 i 1 i 2 2 z 0 i i ∑ 0 i i 2 2 (1) 2 ∂z H(zr2 −Hr1r)h r hi=1 i 1 ai J 0 [aaiihJ0( ai h)] 2 1 i

i

i 1

i 2

where, H isisthe thecoil coilheight, height,HH ρ is the variation in thelift-off, probe where, ⊗ denotes denotesconvolution. convolution. H = z=2 −z2z1.−ρ zis1 .the variation in the probe lift-off, ρ ≥ 0. I(t) and N are the excitation current and number of turns of the excitation coil. is ρ ≥ 0. I(t) and N are the excitation current and number of turns of the excitation coil. μ0 isµ0the the permeability of vacuum. J0 denotes Bessel function. positive 0. The 1 (a=i h) i is the permeability of vacuum. J0 denotes the the Bessel function. ai is athe positive rootroot of J1of (aiJh) 0. =The coil coil coefficient χ(a r , a r ) can be computed by referring to the identity in [17,18]. η (t) stands for 1 2 i i i coefficient χ(air1, air2) can be computed by referring to the identity in [17,18]. ηi(t) stands for the the generalized generalized temporal temporal expression expression of of the the conductor conductor reflection reflection coefficient coefficient [16], [16], and and varies varies with with HMD HMD parameters ). parameters i.e., i.e., the the thickness thickness and and conductivity conductivity of of HMD HMD (d (d11 and and σσ11).

Figure 1. 2D axi-symmetric model of a GPEC probe over a coated nonmagnetic conductor with Figure 1. 2D axi-symmetric model of a GPEC probe over a coated nonmagnetic conductor with HMD. HMD.

Equation Equation (1) (1) facilitates facilitates the the computation computation of of transient transient GPEC GPEC responses responses to to the the coated coated nonmagnetic nonmagnetic conductor conductor with with HMD. HMD. By By referring referring to to the the previous previous study study revealing revealing that that LOI LOI can can only only be be found found in in the the first-order derivatives of the eddy current testing signals against time [11], the first-order derivatives first-order derivatives of the eddy current testing signals against time [11], the first-order of the testingofsignals fromsignals the GPEC against time against are further LOI point could derivatives the testing fromprobe the GPEC probe timeformulated. are further The formulated. The LOI be identified byidentified finding the gz ’(B where: z )|ρ 6= ∞ gand ρ =g∞z’(B point could be byintersection finding the between intersection between z’(Bzg )|z ρ’(B ≠ ∞z )| and z)|ρ = ∞ where: h i a z 0 N I (t ) t∞ ar , a r ' az a ( z 2 ) ai ze1 a z − ai z2 i 1χ (ia2i r1 , ai r2 ) Bz µ0 N{∂[ I (t)]/∂t} ⊗ J0 (Ja0i r)ai reaize− e−e ai (z+2ρ)iη(ti )(t) e e− gz0 ( Bz ) ρ6=g∞z = − e (2) 2 ∑ 2 2 (2) H r1r2) h2r1 h i 1 H (r2 − i =1 ai J 0 [aai ihJ0( ai h)] i

i

i 1

i 2

h t )/∂t t} ∞ iaχr(,aa rr , a r ) µ NN{∂[ I(It()] a ( z z ) 1 ) ai ( z azi2()z − z ' e− e 2 ) i 1 ii 12 2 i 22 JJ00(aai irr) ee ai i (z−1 z 0 0 (3) gz0 ( Bzg)z ρB ∑ (3) 22 =z∞ = HH (r2r− rr11 ) h 1 1 ai J 0[ a iaJi 0h(ai h)] 2 ii= Mloi and Tloi of the identified LOI point, which are invariant to ρ, can be subsequently extracted Mloi and Tloi of the identified LOI point, which are invariant to ρ, can be subsequently extracted for investigation of LOI characteristics of GPEC. It is noted that GPEC probes are mostly driven by the for investigation of LOI characteristics of GPEC. It is noted that GPEC probes are mostly driven by exponential excitation current written as [19]: the exponential excitation current written as [19]: ( −τtt 0, 0, tt